Incommensurate structure of Ca~2~Al~2~O~5~ at high temperatures ‒ structure investigation and Raman spectroscopy
Lazic, Biljana; Krüger, Hannes; Kahlenberg, Volker; Konzett, Jürgen; Kaindl, Reinhard; Acta Crystallographica Section B 64 (2008) 417–425; doi:10.1107/S0108768108016029

data_2104173
_publ_section_title
;
 Incommensurate structure of Ca~2~Al~2~O~5~ at high temperatures --
 structure investigation and Raman spectroscopy
;
_journal_coeditor_code           SN5068
_journal_issue                   4
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              417
_journal_page_last               425
_journal_paper_doi               10.1107/S0108768108016029
_journal_volume                  64
_journal_year                    2008
_chemical_formula_sum            'Al2 Ca2 O5'
_chemical_formula_weight         214.12
_space_group_ssg_name            Imma(00\g)s00
_symmetry_cell_setting           orthorhombic
_audit_creation_method
;
  Jana2000 Version : 18/12/2007
  STOE X-RED
  enCIFer 1.2
;
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   5.2699(5)
_cell_length_b                   14.6984(15)
_cell_length_c                   5.4196(5)
_cell_measurement_reflns_used    3428
_cell_measurement_temperature    1090(10)
_cell_measurement_theta_max      30.82
_cell_measurement_theta_min      2.77
_cell_modulation_dimension       1
_cell_volume                     419.80(7)
_computing_cell_refinement       'STOE X-AREA'
_computing_data_collection       'STOE X-AREA'
_computing_data_reduction        'STOE X-RED'
_computing_publication_material
'Jana2000 (Petricek, Dusek & Palatinus, 2000)'
_computing_structure_refinement
'Jana2000 (Petricek, Dusek & Palatinus, 2000)'
_diffrn_ambient_temperature      1090(10)
_diffrn_detector_area_resol_mean 6.67
_diffrn_measurement_device       '2-circle goniometer'
_diffrn_measurement_device_type  'STOE IPDS 2'
_diffrn_measurement_method       'rotation method'
_diffrn_radiation_monochromator  'plane graphite'
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0530
_diffrn_reflns_av_sigmaI/netI    0.0105
_diffrn_reflns_limit_h_max       7
_diffrn_reflns_limit_h_min       -7
_diffrn_reflns_limit_k_max       20
_diffrn_reflns_limit_k_min       -20
_diffrn_reflns_limit_l_max       7
_diffrn_reflns_limit_l_min       -7
_diffrn_reflns_number            5551
_diffrn_reflns_theta_max         29.13
_diffrn_reflns_theta_min         1.84
_exptl_absorpt_coefficient_mu    3.04
_exptl_absorpt_correction_T_max  0.8340
_exptl_absorpt_correction_T_min  0.7938
_exptl_absorpt_correction_type   integration
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    3.388
_exptl_crystal_description       fragment
_exptl_crystal_F_000             424
_exptl_crystal_size_max          0.14
_exptl_crystal_size_mid          0.12
_exptl_crystal_size_min          0.1
_refine_diff_density_max         1.16
_refine_diff_density_min         -1.04
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   3.52
_refine_ls_number_parameters     43
_refine_ls_number_reflns         848
_refine_ls_R_factor_all          0.0695
_refine_ls_R_factor_gt           0.0546
_refine_ls_shift/su_max          0.0001
_refine_ls_shift/su_mean         0.0000
_refine_ls_structure_factor_coef F
_refine_ls_weighting_details     w=1/(\s^2^(F)+0.0001F^2^)
_refine_ls_weighting_scheme      sigma
_refine_ls_wR_factor_gt          0.0659
_refine_ls_wR_factor_ref         0.0677
_reflns_number_gt                680
_reflns_number_total             848
_reflns_threshold_expression     I>3\s(I)
_cod_data_source_file            sn5068.cif
_cod_data_source_block           I
_cod_original_formula_sum        'Ca2 Al2 O5'
_cod_database_code               2104173
_cod_database_fobs_code          2104173